De Novo Tailoring Pore Morphologies and Sizes for Different Substrates in a Urea-Containing MOFs Catalytic Platform
Ju, Zhanfeng; Yan, Shichen; Yuan, Daqiang; Chemistry of Materials 28 (2016) 2000–; doi:10.1021/acs.chemmater.5b03999

data_4003216
_publ_section_title
;
 De Novo Tailoring Pore Morphologies and Sizes for Different Substrates in
 a Urea-Containing MOFs Catalytic Platform
;
_journal_issue                   7
_journal_name_full               'Chemistry of Materials'
_journal_page_first              2000
_journal_paper_doi               10.1021/acs.chemmater.5b03999
_journal_volume                  28
_journal_year                    2016
_chemical_formula_sum            'C33 H24 Cu3 N6 O18'
_chemical_formula_weight         983.20
_space_group_crystal_system      tetragonal
_space_group_IT_number           87
_space_group_name_Hall           '-I 4'
_space_group_name_H-M_alt        'I 4/m'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            16
_cell_length_a                   30.4638(3)
_cell_length_b                   30.4638(3)
_cell_length_c                   44.2772(7)
_cell_measurement_reflns_used    10241
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      68.4030
_cell_measurement_theta_min      3.3740
_cell_volume                     41091.2(9)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXT-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      100(2)
_diffrn_detector_area_resol_mean 10.5594
_diffrn_measured_fraction_theta_full 0.994
_diffrn_measured_fraction_theta_max 0.965
_diffrn_measurement_device_type  'SuperNova, Dual, Cu at zero, Atlas'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54184
_diffrn_reflns_av_R_equivalents  0.0318
_diffrn_reflns_av_unetI/netI     0.0460
_diffrn_reflns_Laue_measured_fraction_full 0.994
_diffrn_reflns_Laue_measured_fraction_max 0.965
_diffrn_reflns_limit_h_max       37
_diffrn_reflns_limit_h_min       -25
_diffrn_reflns_limit_k_max       34
_diffrn_reflns_limit_k_min       -36
_diffrn_reflns_limit_l_max       54
_diffrn_reflns_limit_l_min       -54
_diffrn_reflns_number            41283
_diffrn_reflns_point_group_measured_fraction_full 0.994
_diffrn_reflns_point_group_measured_fraction_max 0.965
_diffrn_reflns_theta_full        67.684
_diffrn_reflns_theta_max         73.355
_diffrn_reflns_theta_min         3.394
_diffrn_source                   'sealed X-ray tube'
_exptl_absorpt_coefficient_mu    1.009
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.98398
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    0.636
_exptl_crystal_description       prism
_exptl_crystal_F_000             7920
_exptl_crystal_size_max          0.100
_exptl_crystal_size_mid          0.090
_exptl_crystal_size_min          0.080
_refine_diff_density_max         0.792
_refine_diff_density_min         -0.691
_refine_diff_density_rms         0.079
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.974
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     547
_refine_ls_number_reflns         20219
_refine_ls_number_restraints     138
_refine_ls_restrained_S_all      1.108
_refine_ls_R_factor_all          0.1083
_refine_ls_R_factor_gt           0.0764
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1757P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2187
_refine_ls_wR_factor_ref         0.2580
_reflns_Friedel_coverage         0.000
_reflns_number_gt                12212
_reflns_number_total             20219
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            cm5b03999_si_002.cif
_cod_data_source_block           URMOF1
_cod_original_cell_volume        41091.1(10)
_cod_database_code               4003216
_shelx_shelxl_version_number     2014/7
_shelx_estimated_absorpt_t_min   0.906
_shelx_estimated_absorpt_t_max   0.924
_shelx_res_checksum              45192
_shelx_hkl_checksum              80859
_shelx_fab_checksum              54369